#------------------------------------------------------------------------------
#$Date: 2025-07-01 13:52:58 +0300 (Tue, 01 Jul 2025) $
#$Revision: 1142 $
#$URL: svn://crystallography.net/testcod/cif/4/00/00/4000000.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4000000
loop_
_publ_author_name
'Georgieva, Veselina M.'
'Bruce, Elliott L.'
'Chitac, Ruxandra G.'
'Lozinska, Magdalena M.'
'Hall, Anna M.'
'Murray, Claire A.'
'Smith, Ronald I.'
'Turrina, Alessandro'
'Wright, Paul A.'
_publ_section_title
;
 Cation Control of Cooperative CO2 Adsorption in Li-Containing Mixed
 Cation Forms of the Flexible Zeolite Merlinoite
;
_journal_issue                   4
_journal_name_full               'Chemistry of Materials'
_journal_page_first              1157
_journal_page_last               1173
_journal_paper_doi               10.1021/acs.chemmater.0c03773
_journal_volume                  33
_journal_year                    2021
_chemical_formula_moiety         'Al6.08 O64 Si25.92, 6Li'
_chemical_formula_structural     'Al6.08 Li6 O64 Si25.92'
_chemical_formula_sum            'Al6.08 Li6 O64 Si25.92'
_chemical_formula_weight         1957.77
_space_group_IT_number           71
_space_group_name_Hall           '-I 2 2'
_space_group_name_H-M_alt        'I m m m'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-I 2 2'
_symmetry_space_group_name_H-M   'I m m m'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            1
_cell_length_a                   13.1589(11)
_cell_length_b                   13.0652(10)
_cell_length_c                   9.9754(8)
_cell_measurement_temperature    298
_cell_volume                     1715.0(2)
_diffrn_ambient_temperature      298
_diffrn_measurement_device_type  Polaris
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    1.896
_exptl_crystal_F_000             971.9
_pd_block_id                     2021-01-05T13:24|5C_phase1|magda||
_pd_phase_name                   'from C:/GSAS/MyWork/MML849+932/LiRho.cif'
_refine_ls_shift/su_max          0.06
_cod_data_source_file            cm0c03773_si_003.cif
_cod_data_source_block           5C_phase_1
_cod_original_cell_volume        1715.01(34)
_cod_database_code               4000000
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 -x,+y,+z
3 +x,-y,+z
4 -x,-y,+z
-1 -x,-y,-z
-2 +x,-y,-z
-3 -x,+y,-z
-4 +x,+y,-z
101 +x+1/2,+y+1/2,+z+1/2
102 -x+1/2,+y+1/2,+z+1/2
103 +x+1/2,-y+1/2,+z+1/2
104 -x+1/2,-y+1/2,+z+1/2
-101 -x+1/2,-y+1/2,-z+1/2
-102 +x+1/2,-y+1/2,-z+1/2
-103 -x+1/2,+y+1/2,-z+1/2
-104 +x+1/2,+y+1/2,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
O O1 0.19818(17) 0.12299(21) 0.18144(25) 1.0 Uiso 0.02809(13) 16
O O2 0.11589(31) 0.25118(23) 0.0 1.0 Uiso 0.02809(13) 8
O O5 0.65673(30) 0.14023(30) 0.0 1.0 Uiso 0.02809(13) 8
O O3 0.0 0.14575(24) 0.1812(4) 1.0 Uiso 0.02809(13) 8
O O6 0.64458(26) 0.0 0.20830(33) 1.0 Uiso 0.02809(13) 8
O O4 0.11777(22) 0.30869(20) 0.25480(30) 1.0 Uiso 0.02809(13) 16
Si Si1 0.1121(4) 0.20926(28) 0.14831(30) 0.81 Uiso 0.02809(13) 16
Al Al1 0.1121(4) 0.20926(28) 0.14831(30) 0.19 Uiso 0.02809(13) 16
Si Si2 0.67539(27) 0.11046(28) 0.1549(4) 0.81 Uiso 0.02809(13) 16
Al Al2 0.67539(27) 0.11046(28) 0.1549(4) 0.19 Uiso 0.02809(13) 16
Li Li1 0.4188(13) 0.5 0.3026(13) 0.551(15) Uiso 0.01 8
Li Li2 0.5 0.1841(35) 0.395(4) 0.199(16) Uiso 0.01 8
loop_
_atom_type_symbol
_atom_type_number_in_cell
O 64.0
Si 25.92
Al 6.08
Li 5.996
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Si1 O1 Al1 0.0 1_555 . 1_555 N
Si1 O1 Si2 135.85(23) 1_555 . 2_655 N
Si1 O1 Al2 135.85(23) 1_555 . 2_655 N
Si1 O1 Li1 91.9(4) 1_555 . -101_555 N
Al1 O1 Si2 135.85(23) 1_555 . 2_655 N
Al1 O1 Al2 135.85(23) 1_555 . 2_655 N
Al1 O1 Li1 91.9(4) 1_555 . -101_555 N
Si2 O1 Al2 0.0 2_655 . 2_655 N
Si2 O1 Li1 128.3(4) 2_655 . -101_555 N
Al2 O1 Li1 128.3(4) 2_655 . -101_555 N
Si1 O2 Si1 139.22(31) 1_555 . -4_555 N
Si1 O2 Al1 0.0 1_555 . 1_555 N
Si1 O2 Al1 139.22(31) 1_555 . -4_555 N
Si1 O2 Li2 127.0(9) 1_555 . 103_454 N
Si1 O2 Li2 68.8(12) 1_555 . -101_555 N
Si1 O2 Al1 139.22(31) -4_555 . 1_555 N
Si1 O2 Al1 0.0 -4_555 . -4_555 N
Si1 O2 Li2 68.8(12) -4_555 . 103_454 N
Si1 O2 Li2 127.0(9) -4_555 . -101_555 N
Al1 O2 Al1 139.22(31) 1_555 . -4_555 N
Al1 O2 Li2 127.0(9) 1_555 . 103_454 N
Al1 O2 Li2 68.8(12) 1_555 . -101_555 N
Al1 O2 Li2 68.8(12) -4_555 . 103_454 N
Al1 O2 Li2 127.0(9) -4_555 . -101_555 N
Li2 O2 Li2 61.8(20) 103_454 . -101_555 N
Si2 O5 Si2 146.85(35) 1_555 . -4_555 N
Si2 O5 Al2 0.0 1_555 . 1_555 N
Si2 O5 Al2 146.85(35) 1_555 . -4_555 N
Si2 O5 Al2 146.85(35) -4_555 . 1_555 N
Si2 O5 Al2 0.0 -4_555 . -4_555 N
Al2 O5 Al2 146.85(35) 1_555 . -4_555 N
Si1 O3 Si1 117.66(32) 1_555 . 2_555 N
Si1 O3 Al1 0.0 1_555 . 1_555 N
Si1 O3 Al1 117.66(32) 1_555 . 2_555 N
Si1 O3 Li1 90.9(4) 1_555 . -101_555 N
Si1 O3 Li1 148.2(4) 1_555 . -102_455 N
Si1 O3 Li2 58.87(16) 1_555 . -101_555 N
Si1 O3 Al1 117.66(32) 2_555 . 1_555 N
Si1 O3 Al1 0.0 2_555 . 2_555 N
Si1 O3 Li1 148.2(4) 2_555 . -101_555 N
Si1 O3 Li1 90.9(4) 2_555 . -102_455 N
Si1 O3 Li2 58.87(16) 2_555 . -101_555 N
Al1 O3 Al1 117.66(32) 1_555 . 2_555 N
Al1 O3 Li1 90.9(4) 1_555 . -101_555 N
Al1 O3 Li1 148.2(4) 1_555 . -102_455 N
Al1 O3 Li2 58.87(16) 1_555 . -101_555 N
Al1 O3 Li1 148.2(4) 2_555 . -101_555 N
Al1 O3 Li1 90.9(4) 2_555 . -102_455 N
Al1 O3 Li2 58.87(16) 2_555 . -101_555 N
Li1 O3 Li1 58.4(8) -101_555 . -102_455 N
Li1 O3 Li2 147.9(6) -101_555 . -101_555 N
Li1 O3 Li2 147.9(6) -102_455 . -101_555 N
Si2 O6 Si2 130.2(4) 1_555 . 3_555 N
Si2 O6 Al2 0.0 1_555 . 1_555 N
Si2 O6 Al2 130.2(4) 1_555 . 3_555 N
Si2 O6 Al2 130.2(4) 3_555 . 1_555 N
Si2 O6 Al2 0.0 3_555 . 3_555 N
Al2 O6 Al2 130.2(4) 1_555 . 3_555 N
Si1 O4 Al1 0.0 1_555 . 1_555 N
Si1 O4 Si2 153.87(32) 1_555 . -102_455 N
Si1 O4 Al2 153.87(32) 1_555 . -102_455 N
Si1 O4 Li2 64.1(12) 1_555 . -101_555 N
Al1 O4 Si2 153.87(32) 1_555 . -102_455 N
Al1 O4 Al2 153.87(32) 1_555 . -102_455 N
Al1 O4 Li2 64.1(12) 1_555 . -101_555 N
Si2 O4 Al2 0.0 -102_455 . -102_455 N
Si2 O4 Li2 135.3(12) -102_455 . -101_555 N
Al2 O4 Li2 135.3(12) -102_455 . -101_555 N
O1 Si1 O2 114.05(31) 1_555 . 1_555 N
O1 Si1 O3 102.88(21) 1_555 . 1_555 N
O1 Si1 O4 112.04(29) 1_555 . 1_555 N
O1 Si1 Li1 52.6(4) 1_555 . -101_555 N
O1 Si1 Li2 178.5(10) 1_555 . -101_555 N
O2 Si1 O3 111.9(4) 1_555 . 1_555 N
O2 Si1 O4 108.85(26) 1_555 . 1_555 N
O2 Si1 Li1 120.41(30) 1_555 . -101_555 N
O2 Si1 Li2 66.0(10) 1_555 . -101_555 N
O3 Si1 O4 106.85(25) 1_555 . 1_555 N
O3 Si1 Li1 51.2(4) 1_555 . -101_555 N
O3 Si1 Li2 75.8(9) 1_555 . -101_555 N
O4 Si1 Li1 130.48(33) 1_555 . -101_555 N
O4 Si1 Li2 69.2(11) 1_555 . -101_555 N
Li1 Si1 Li2 126.0(9) -101_555 . -101_555 N
O1 Al1 O2 114.05(31) 1_555 . 1_555 N
O1 Al1 O3 102.88(21) 1_555 . 1_555 N
O1 Al1 O4 112.04(29) 1_555 . 1_555 N
O1 Al1 Li1 52.6(4) 1_555 . -101_555 N
O1 Al1 Li2 178.5(10) 1_555 . -101_555 N
O2 Al1 O3 111.9(4) 1_555 . 1_555 N
O2 Al1 O4 108.85(26) 1_555 . 1_555 N
O2 Al1 Li1 120.41(30) 1_555 . -101_555 N
O2 Al1 Li2 66.0(10) 1_555 . -101_555 N
O3 Al1 O4 106.85(25) 1_555 . 1_555 N
O3 Al1 Li1 51.2(4) 1_555 . -101_555 N
O3 Al1 Li2 75.8(9) 1_555 . -101_555 N
O4 Al1 Li1 130.48(33) 1_555 . -101_555 N
O4 Al1 Li2 69.2(11) 1_555 . -101_555 N
Li1 Al1 Li2 126.0(9) -101_555 . -101_555 N
O1 Si2 O5 106.03(25) 2_655 . 1_555 N
O1 Si2 O6 106.62(22) 2_655 . 1_555 N
O1 Si2 O4 108.52(25) 2_655 . -102_555 N
O5 Si2 O6 120.06(33) 1_555 . 1_555 N
O5 Si2 O4 108.16(25) 1_555 . -102_555 N
O6 Si2 O4 107.04(32) 1_555 . -102_555 N
O1 Al2 O5 106.03(25) 2_655 . 1_555 N
O1 Al2 O6 106.62(22) 2_655 . 1_555 N
O1 Al2 O4 108.52(25) 2_655 . -102_555 N
O5 Al2 O6 120.06(33) 1_555 . 1_555 N
O5 Al2 O4 108.16(25) 1_555 . -102_555 N
O6 Al2 O4 107.04(32) 1_555 . -102_555 N
O1 Li1 O1 92.1(7) -101_444 . -103_444 N
O1 Li1 O3 72.84(12) -101_444 . -101_444 N
O1 Li1 O3 163.3(7) -101_444 . -103_444 N
O1 Li1 Si1 35.52(13) -101_555 . -101_555 N
O1 Li1 Si1 126.1(7) -101_555 . -103_555 N
O1 Li1 Al1 35.52(13) -101_555 . -101_555 N
O1 Li1 Al1 126.1(7) -101_555 . -103_555 N
O1 Li1 Li1 133.64(34) -101_555 . 2_655 N
O1 Li1 O3 163.3(7) -103_444 . -101_444 N
O1 Li1 O3 72.84(12) -103_444 . -103_444 N
O1 Li1 Si1 126.1(7) -103_555 . -101_555 N
O1 Li1 Si1 35.52(13) -103_555 . -103_555 N
O1 Li1 Al1 126.1(7) -103_555 . -101_555 N
O1 Li1 Al1 35.52(13) -103_555 . -103_555 N
O1 Li1 Li1 133.64(34) -103_555 . 2_655 N
O3 Li1 O3 120.9(8) -101_444 . -103_444 N
O3 Li1 Si1 37.88(12) -101_555 . -101_555 N
O3 Li1 Si1 154.8(7) -101_555 . -103_555 N
O3 Li1 Al1 37.88(12) -101_555 . -101_555 N
O3 Li1 Al1 154.8(7) -101_555 . -103_555 N
O3 Li1 Li1 60.8(4) -101_555 . 2_655 N
O3 Li1 Si1 154.8(7) -103_555 . -101_555 N
O3 Li1 Si1 37.88(12) -103_555 . -103_555 N
O3 Li1 Al1 154.8(7) -103_555 . -101_555 N
O3 Li1 Al1 37.88(12) -103_555 . -103_555 N
O3 Li1 Li1 60.8(4) -103_555 . 2_655 N
Si1 Li1 Si1 153.8(6) -101_555 . -103_555 N
Si1 Li1 Al1 0.0 -101_555 . -101_555 N
Si1 Li1 Al1 153.8(6) -101_555 . -103_555 N
Si1 Li1 Li1 98.3(4) -101_555 . 2_655 N
Si1 Li1 Al1 153.8(6) -103_555 . -101_555 N
Si1 Li1 Al1 0.0 -103_555 . -103_555 N
Si1 Li1 Li1 98.3(4) -103_555 . 2_655 N
Al1 Li1 Al1 153.8(6) -101_555 . -103_555 N
Al1 Li1 Li1 98.3(4) -101_555 . 2_655 N
Al1 Li1 Li1 98.3(4) -103_555 . 2_655 N
O2 Li2 O2 97.2(17) 103_555 . 104_555 N
O2 Li2 O3 76.9(14) 103_555 . -101_444 N
O2 Li2 O4 151.4(24) 103_555 . -101_555 N
O2 Li2 O4 78.4(5) 103_555 . -102_555 N
O2 Li2 Si1 111.2(20) 103_555 . -101_555 N
O2 Li2 Si1 45.2(6) 103_555 . -102_555 N
O2 Li2 Al1 111.2(20) 103_555 . -101_555 N
O2 Li2 Al1 45.2(6) 103_555 . -102_555 N
O2 Li2 Li2 59.1(10) 103_555 . -3_656 N
O2 Li2 O3 76.9(14) 104_555 . -101_444 N
O2 Li2 O4 78.4(5) 104_555 . -101_555 N
O2 Li2 O4 151.4(24) 104_555 . -102_555 N
O2 Li2 Si1 45.2(6) 104_555 . -101_555 N
O2 Li2 Si1 111.2(20) 104_555 . -102_555 N
O2 Li2 Al1 45.2(6) 104_555 . -101_555 N
O2 Li2 Al1 111.2(20) 104_555 . -102_555 N
O2 Li2 Li2 59.1(10) 104_555 . -3_656 N
O3 Li2 O4 74.5(12) -101_555 . -101_555 N
O3 Li2 O4 74.5(12) -101_555 . -102_555 N
O3 Li2 Si1 45.3(9) -101_555 . -101_555 N
O3 Li2 Si1 45.3(9) -101_555 . -102_555 N
O3 Li2 Al1 45.3(9) -101_555 . -101_555 N
O3 Li2 Al1 45.3(9) -101_555 . -102_555 N
O3 Li2 Li2 109.0(10) -101_555 . -3_656 N
O4 Li2 O4 91.9(15) -101_555 . -102_555 N
O4 Li2 Si1 46.7(6) -101_555 . -101_555 N
O4 Li2 Si1 109.6(19) -101_555 . -102_555 N
O4 Li2 Al1 46.7(6) -101_555 . -101_555 N
O4 Li2 Al1 109.6(19) -101_555 . -102_555 N
O4 Li2 Li2 134.0(7) -101_555 . -3_656 N
O4 Li2 Si1 109.6(19) -102_555 . -101_555 N
O4 Li2 Si1 46.7(6) -102_555 . -102_555 N
O4 Li2 Al1 109.6(19) -102_555 . -101_555 N
O4 Li2 Al1 46.7(6) -102_555 . -102_555 N
O4 Li2 Li2 134.0(7) -102_555 . -3_656 N
Si1 Li2 Si1 90.6(18) -101_555 . -102_555 N
Si1 Li2 Al1 0.0 -101_555 . -101_555 N
Si1 Li2 Al1 90.6(18) -101_555 . -102_555 N
Si1 Li2 Li2 102.1(10) -101_555 . -3_656 N
Si1 Li2 Al1 90.6(18) -102_555 . -101_555 N
Si1 Li2 Al1 0.0 -102_555 . -102_555 N
Si1 Li2 Li2 102.1(10) -102_555 . -3_656 N
Al1 Li2 Al1 90.6(18) -101_555 . -102_555 N
Al1 Li2 Li2 102.1(10) -101_555 . -3_656 N
Al1 Li2 Li2 102.1(10) -102_555 . -3_656 N
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O1 Si1 1.632(5) . 1_555 N
O1 Al1 1.632(5) . 1_555 N
O1 Si2 1.693(4) . 2_655 N
O1 Al2 1.693(4) . 2_655 N
O1 Li1 2.231(13) . -101_444 N
O2 Si1 1.5783(33) . 1_555 N
O2 Si1 1.5783(33) . -4_555 N
O2 Al1 1.5783(33) . 1_555 N
O2 Al1 1.5783(33) . -4_555 N
O2 Li2 2.032(27) . 103_454 N
O2 Li2 2.032(27) . -101_444 N
O5 Si2 1.612(4) . 1_555 N
O5 Si2 1.612(4) . -4_555 N
O5 Al2 1.612(4) . 1_555 N
O5 Al2 1.612(4) . -4_555 N
O3 Si1 1.724(4) . 1_555 N
O3 Si1 1.724(4) . 2_555 N
O3 Al1 1.724(4) . 1_555 N
O3 Al1 1.724(4) . 2_555 N
O3 Li1 2.189(9) . -101_444 N
O3 Li1 2.189(9) . -102_344 N
O3 Li2 2.35(5) . -101_444 N
O6 Si2 1.591(4) . 1_555 N
O6 Si2 1.591(4) . 3_555 N
O6 Al2 1.591(4) . 1_555 N
O6 Al2 1.591(4) . 3_555 N
O4 Si1 1.680(4) . 1_555 N
O4 Al1 1.680(4) . 1_555 N
O4 Si2 1.582(4) . -102_344 N
O4 Al2 1.582(4) . -102_344 N
O4 Li2 2.157(27) . -101_444 N
Si1 O1 1.632(5) . 1_555 N
Si1 O2 1.5783(33) . 1_555 N
Si1 O3 1.724(4) . 1_555 N
Si1 O4 1.680(4) . 1_555 N
Si1 Si1 2.950(10) . 2_555 N
Si1 Si1 2.959(6) . -4_555 N
Si1 Al1 2.950(10) . 2_555 N
Si1 Al1 2.959(6) . -4_555 N
Si1 Al2 3.081(6) . 2_655 N
Si1 Li1 2.807(5) . -101_444 N
Si1 Li2 3.24(4) . 103_454 N
Si1 Li2 2.075(33) . -101_444 N
Al1 O1 1.632(5) . 1_555 N
Al1 O2 1.5783(33) . 1_555 N
Al1 O3 1.724(4) . 1_555 N
Al1 O4 1.680(4) . 1_555 N
Al1 Si1 2.950(10) . 2_555 N
Al1 Si1 2.959(6) . -4_555 N
Al1 Al1 2.950(10) . 2_555 N
Al1 Al1 2.959(6) . -4_555 N
Al1 Si2 3.081(6) . 2_655 N
Al1 Al2 3.081(6) . 2_655 N
Al1 Al2 3.177(5) . -102_344 N
Al1 Li1 2.807(5) . -101_444 N
Al1 Li2 3.24(4) . 103_454 N
Al1 Li2 2.075(33) . -101_444 N
Si2 O1 1.693(4) . 2_655 N
Si2 O5 1.612(4) . 1_555 N
Si2 O6 1.591(4) . 1_555 N
Si2 O4 1.582(4) . -102_444 N
Si2 Al1 3.081(6) . 2_655 N
Si2 Si2 2.886(7) . 3_555 N
Si2 Al2 2.886(7) . 3_555 N
Si2 Al2 3.091(8) . -4_555 N
Al2 O1 1.693(4) . 2_655 N
Al2 O5 1.612(4) . 1_555 N
Al2 O6 1.591(4) . 1_555 N
Al2 O4 1.582(4) . -102_444 N
Al2 Si1 3.081(6) . 2_655 N
Al2 Al1 3.081(6) . 2_655 N
Al2 Al1 3.177(5) . -102_444 N
Al2 Si2 2.886(7) . 3_555 N
Al2 Si2 3.091(8) . -4_555 N
Al2 Al2 2.886(7) . 3_555 N
Al2 Al2 3.091(8) . -4_555 N
Li1 O1 2.231(13) . -101_444 N
Li1 O1 2.231(13) . -103_444 N
Li1 O3 2.189(9) . -101_444 N
Li1 O3 2.189(9) . -103_444 N
Li1 Si1 2.807(5) . -101_444 N
Li1 Si1 2.807(5) . -103_444 N
Li1 Al1 2.807(5) . -101_444 N
Li1 Al1 2.807(5) . -103_444 N
Li1 Li1 2.14(4) . 2_655 N
Li2 O2 2.032(27) . 103_555 N
Li2 O2 2.032(27) . 104_555 N
Li2 O3 2.35(5) . -101_444 N
Li2 O4 2.157(27) . -101_444 N
Li2 O4 2.157(27) . -102_444 N
Li2 Si1 3.24(4) . 103_555 N
Li2 Si1 3.24(4) . 104_555 N
Li2 Si1 2.075(33) . -101_444 N
Li2 Si1 2.075(33) . -102_444 N
Li2 Al1 3.24(4) . 103_555 N
Li2 Al1 3.24(4) . 104_555 N
Li2 Al1 2.075(33) . -101_444 N
Li2 Al1 2.075(33) . -102_444 N
Li2 Li2 2.09(8) . -3_656 N
loop_
_pd_block_diffractogram_id
2021-01-05T13:24|5C_H_01|magda|g
2021-01-05T13:24|5C_H_02|magda|g
2021-01-05T13:24|5C_H_03|magda|g

_cod_database_fobs_code 4000000
